#------------------------------------------------------------------------------
#$Date: 2016-02-18 17:37:37 +0200 (Thu, 18 Feb 2016) $
#$Revision: 176729 $
#$URL: svn://www.crystallography.net/cod/cif/1/51/71/1517130.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_1517130
loop_
_publ_author_name
'Shu-Yun Shi'
'Zhan-Lin Xu'
'Hong-Hui Teng'
'Ling-Zi Zhao'
'Xiao-Bing Cui'
'Ji-Qing Xu'
_publ_section_title
;
 Two new compounds constructed from polyoxoanions, metal ions and organic
 ligands
;
_journal_name_full
;
Inorganica Chimica Acta
;
_journal_page_first              123
_journal_page_last               127
_journal_volume                  402
_journal_year                    2013
_chemical_formula_sum            'C30 H26 Cu2 Mo12 N6 O40 Si'
_chemical_formula_weight         2417.02
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_cell_angle_alpha                105.386(6)
_cell_angle_beta                 102.406(5)
_cell_angle_gamma                115.660(4)
_cell_formula_units_Z            1
_cell_length_a                   10.8645(9)
_cell_length_b                   11.8169(12)
_cell_length_c                   13.3176(10)
_cell_measurement_temperature    293(2)
_cell_volume                     1374.8(2)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.985
_diffrn_measured_fraction_theta_max 0.985
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0667
_diffrn_reflns_av_sigmaI/netI    0.0603
_diffrn_reflns_limit_h_max       14
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -17
_diffrn_reflns_number            10084
_diffrn_reflns_theta_full        28.38
_diffrn_reflns_theta_max         28.38
_diffrn_reflns_theta_min         1.71
_exptl_absorpt_coefficient_mu    3.524
_exptl_absorpt_correction_T_max  0.5249
_exptl_absorpt_correction_T_min  0.3893
_exptl_absorpt_correction_type   empirical
_exptl_crystal_density_diffrn    2.919
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             1144
_exptl_crystal_size_max          0.33
_exptl_crystal_size_mid          0.23
_exptl_crystal_size_min          0.21
_refine_diff_density_max         6.915
_refine_diff_density_min         -1.950
_refine_diff_density_rms         0.261
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.116
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     430
_refine_ls_number_reflns         6796
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.116
_refine_ls_R_factor_all          0.0866
_refine_ls_R_factor_gt           0.0691
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0726P)²+19.6419P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1749
_refine_ls_wR_factor_ref         0.1881
_reflns_number_gt                5398
_reflns_number_total             6796
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ICA-2013-402-123-127-2.cif
_cod_data_source_block           hh
_cod_original_sg_symbol_H-M      p-1
_cod_database_code               1517130
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, -z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Mo1 Mo 1.09010(10) 0.82527(9) 0.29764(7) 0.0321(2) Uani 1 1 d .
Mo2 Mo 0.72296(10) 0.75134(9) 0.23576(7) 0.0335(2) Uani 1 1 d .
Mo3 Mo 1.13809(11) 0.79190(10) 0.55450(8) 0.0369(2) Uani 1 1 d .
Mo4 Mo 0.99819(10) 1.07089(11) 0.25812(8) 0.0369(2) Uani 1 1 d .
Mo5 Mo 0.62570(9) 0.89055(10) 0.45294(8) 0.0358(2) Uani 1 1 d .
Mo6 Mo 0.75430(10) 0.66490(9) 0.47204(8) 0.0360(2) Uani 1 1 d .
Si1 Si 1.0000 1.0000 0.5000 0.0173(6) Uani 1 2 d S
O1 O 0.9640(13) 0.9340(13) 0.3672(10) 0.023(2) Uani 0.50 1 d P
O2 O 1.1127(12) 0.9487(12) 0.4805(9) 0.019(2) Uani 0.50 1 d P
O3 O 0.8296(13) 0.8687(13) 0.4334(10) 0.025(2) Uani 0.50 1 d P
O4 O 1.0207(14) 1.1161(13) 0.4490(10) 0.026(2) Uani 0.50 1 d P
O5 O 1.0860(10) 0.9691(12) 0.2436(13) 0.086(4) Uani 1 1 d .
O6 O 0.5957(9) 0.6265(9) 0.1099(7) 0.052(2) Uani 1 1 d .
O7 O 1.1416(11) 0.7562(10) 0.2013(7) 0.052(2) Uani 1 1 d .
O8 O 0.6366(11) 0.5118(9) 0.4626(10) 0.062(3) Uani 1 1 d .
O9 O 1.3081(14) 0.9469(10) 0.5879(7) 0.088(4) Uani 1 1 d .
O10 O 0.8894(10) 0.7242(11) 0.2267(13) 0.086(4) Uani 1 1 d .
O11 O 0.8072(11) 0.8970(11) 0.1982(13) 0.083(4) Uani 1 1 d .
O12 O 1.1037(14) 0.7436(11) 0.3929(8) 0.092(5) Uani 1 1 d .
O13 O 0.7132(14) 1.0085(10) 0.5997(8) 0.083(4) Uani 1 1 d .
O14 O 0.7043(18) 0.6358(15) 0.3229(10) 0.094(5) Uani 1 1 d .
O15 O 1.1196(10) 0.8553(14) 0.6891(9) 0.089(4) Uani 1 1 d .
O16 O 0.9216(11) 0.6643(15) 0.4885(10) 0.107(6) Uani 1 1 d .
O17 O 0.9882(11) 1.0993(11) 0.1424(8) 0.061(3) Uani 1 1 d .
O18 O 0.6156(18) 0.8065(15) 0.2981(9) 0.096(5) Uani 1 1 d .
O19 O 0.4502(9) 0.8402(12) 0.4229(8) 0.062(3) Uani 1 1 d .
O20 O 1.1670(11) 1.2290(15) 0.3618(9) 0.096(5) Uani 1 1 d .
O21 O 0.6290(19) 0.7491(15) 0.4793(10) 0.096(5) Uani 1 1 d .
O22 O 1.1962(11) 0.6884(10) 0.5725(7) 0.053(2) Uani 1 1 d .
Cu1 Cu 0.49347(16) 0.39980(18) 0.14372(18) 0.0621(5) Uani 1 1 d .
N1 N 0.3194(10) 0.3973(10) 0.1498(10) 0.048(2) Uani 1 1 d .
N2 N 0.6581(10) 0.3839(10) 0.1353(9) 0.042(2) Uani 1 1 d .
N3 N 0.3356(18) 0.047(2) 0.1947(17) 0.109(7) Uani 1 1 d .
C1 C 0.1906(12) 0.4795(13) 0.2426(10) 0.046(3) Uani 1 1 d .
H1 H 0.1942 0.5348 0.3090 0.055 Uiso 1 1 calc R
C2 C 0.0639(10) 0.4038(10) 0.1451(9) 0.0297(19) Uani 1 1 d .
C3 C 0.3119(13) 0.4691(15) 0.2366(13) 0.062(4) Uani 1 1 d .
H3 H 0.3961 0.5193 0.3023 0.075 Uiso 1 1 calc R
C4 C 0.0682(13) 0.3237(15) 0.0493(10) 0.046(3) Uani 1 1 d .
H4 H -0.0145 0.2704 -0.0175 0.056 Uiso 1 1 calc R
C5 C 0.1977(13) 0.3245(14) 0.0552(9) 0.045(3) Uani 1 1 d .
H5 H 0.2001 0.2722 -0.0093 0.053 Uiso 1 1 calc R
C6 C 0.6984(13) 0.3804(15) 0.0467(11) 0.051(3) Uani 1 1 d .
H6 H 0.6362 0.3747 -0.0170 0.061 Uiso 1 1 calc R
C7 C 0.8277(12) 0.3849(14) 0.0446(10) 0.045(3) Uani 1 1 d .
H7 H 0.8491 0.3789 -0.0199 0.054 Uiso 1 1 calc R
C8 C 0.9246(10) 0.3986(11) 0.1408(8) 0.032(2) Uani 1 1 d .
C9 C 0.8870(11) 0.4096(11) 0.2351(9) 0.034(2) Uani 1 1 d .
H9 H 0.9511 0.4238 0.3023 0.041 Uiso 1 1 calc R
C10 C 0.288(3) 0.049(3) 0.098(2) 0.122(10) Uani 1 1 d .
H10 H 0.2110 0.0644 0.0813 0.146 Uiso 1 1 calc R
C11 C 0.4660(14) 0.0075(19) 0.0400(16) 0.083(6) Uani 1 1 d .
C12 C 0.346(2) 0.029(3) 0.021(2) 0.109(9) Uani 1 1 d .
H12 H 0.3053 0.0284 -0.0486 0.131 Uiso 1 1 calc R
C13 C 0.5172(18) 0.015(3) 0.1497(18) 0.110(9) Uani 1 1 d .
H13 H 0.6014 0.0107 0.1732 0.132 Uiso 1 1 calc R
C14 C 0.452(2) 0.028(3) 0.219(2) 0.122(10) Uani 1 1 d .
H14 H 0.4857 0.0241 0.2876 0.147 Uiso 1 1 calc R
C15 C 0.7524(12) 0.3989(11) 0.2276(10) 0.039(2) Uani 1 1 d .
H15 H 0.7270 0.4025 0.2902 0.046 Uiso 1 1 calc R
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O7 Mo1 O12 102.2(6) . .
O7 Mo1 O10 101.6(6) . .
O12 Mo1 O10 97.3(5) . .
O7 Mo1 O13 98.5(5) . 2_776
O12 Mo1 O13 90.2(4) . 2_776
O10 Mo1 O13 156.4(6) . 2_776
O7 Mo1 O5 97.1(5) . .
O12 Mo1 O5 158.7(6) . .
O10 Mo1 O5 87.2(4) . .
O13 Mo1 O5 78.2(5) 2_776 .
O7 Mo1 O2 156.9(4) . .
O12 Mo1 O2 66.5(5) . .
O10 Mo1 O2 99.9(6) . .
O13 Mo1 O2 62.8(5) 2_776 .
O5 Mo1 O2 92.3(5) . .
O7 Mo1 O1 155.2(4) . .
O12 Mo1 O1 100.2(6) . .
O10 Mo1 O1 65.1(5) . .
O13 Mo1 O1 91.6(5) 2_776 .
O5 Mo1 O1 62.8(5) . .
O2 Mo1 O1 45.8(4) . .
O6 Mo2 O18 102.5(6) . .
O6 Mo2 O11 101.3(6) . .
O18 Mo2 O11 95.8(5) . .
O6 Mo2 O14 98.3(6) . .
O18 Mo2 O14 88.3(4) . .
O11 Mo2 O14 158.7(6) . .
O6 Mo2 O10 97.5(5) . .
O18 Mo2 O10 158.8(6) . .
O11 Mo2 O10 87.3(4) . .
O14 Mo2 O10 81.7(5) . .
O6 Mo2 O3 157.0(5) . .
O18 Mo2 O3 64.9(5) . .
O11 Mo2 O3 99.2(6) . .
O14 Mo2 O3 63.6(5) . .
O10 Mo2 O3 93.9(5) . .
O6 Mo2 O1 155.9(4) . .
O18 Mo2 O1 98.7(6) . .
O11 Mo2 O1 64.9(5) . .
O14 Mo2 O1 93.8(6) . .
O10 Mo2 O1 63.7(5) . .
O3 Mo2 O1 46.0(4) . .
O22 Mo3 O9 102.0(6) . .
O22 Mo3 O15 101.9(6) . .
O9 Mo3 O15 95.1(5) . .
O22 Mo3 O16 101.2(6) . .
O9 Mo3 O16 155.5(7) . .
O15 Mo3 O16 87.5(5) . .
O22 Mo3 O12 97.9(5) . .
O9 Mo3 O12 89.0(4) . .
O15 Mo3 O12 158.5(6) . .
O16 Mo3 O12 80.4(5) . .
O22 Mo3 O4 156.5(5) . 2_776
O9 Mo3 O4 98.5(6) . 2_776
O15 Mo3 O4 64.8(5) . 2_776
O16 Mo3 O4 60.7(5) . 2_776
O12 Mo3 O4 93.8(6) . 2_776
O22 Mo3 O2 156.1(4) . .
O9 Mo3 O2 64.5(5) . .
O15 Mo3 O2 99.0(6) . .
O16 Mo3 O2 91.0(6) . .
O12 Mo3 O2 63.8(5) . .
O4 Mo3 O2 46.3(4) 2_776 .
O17 Mo4 O20 101.4(6) . .
O17 Mo4 O5 100.8(6) . .
O20 Mo4 O5 94.3(5) . .
O17 Mo4 O11 98.9(5) . .
O20 Mo4 O11 158.7(6) . .
O5 Mo4 O11 87.9(4) . .
O17 Mo4 O15 99.5(6) . 2_776
O20 Mo4 O15 89.5(4) . 2_776
O5 Mo4 O15 158.1(6) . 2_776
O11 Mo4 O15 81.0(5) . 2_776
O17 Mo4 O4 157.3(5) . .
O20 Mo4 O4 65.6(5) . .
O5 Mo4 O4 98.8(5) . .
O11 Mo4 O4 93.2(5) . .
O15 Mo4 O4 63.4(5) 2_776 .
O17 Mo4 O1 156.0(5) . .
O20 Mo4 O1 99.1(6) . .
O5 Mo4 O1 65.2(5) . .
O11 Mo4 O1 62.7(5) . .
O15 Mo4 O1 93.0(5) 2_776 .
O4 Mo4 O1 46.0(4) . .
O19 Mo5 O21 100.8(6) . .
O19 Mo5 O13 103.4(6) . .
O21 Mo5 O13 95.2(5) . .
O19 Mo5 O18 98.9(6) . .
O21 Mo5 O18 88.9(4) . .
O13 Mo5 O18 156.2(7) . .
O19 Mo5 O9 99.9(6) . 2_776
O21 Mo5 O9 157.4(6) . 2_776
O13 Mo5 O9 88.6(4) . 2_776
O18 Mo5 O9 79.2(5) . 2_776
O19 Mo5 O3 155.5(5) . .
O21 Mo5 O3 65.9(5) . .
O13 Mo5 O3 98.5(6) . .
O18 Mo5 O3 61.8(5) . .
O9 Mo5 O3 91.5(5) 2_776 .
O19 Mo5 O2 156.9(5) . 2_776
O21 Mo5 O2 99.7(6) . 2_776
O13 Mo5 O2 64.2(5) . 2_776
O18 Mo5 O2 91.9(6) . 2_776
O9 Mo5 O2 62.0(5) 2_776 2_776
O3 Mo5 O2 46.2(4) . 2_776
O8 Mo6 O16 103.8(7) . .
O8 Mo6 O14 100.9(6) . .
O16 Mo6 O14 95.8(6) . .
O8 Mo6 O20 99.5(6) . 2_776
O16 Mo6 O20 88.8(5) . 2_776
O14 Mo6 O20 157.3(6) . 2_776
O8 Mo6 O21 99.0(6) . .
O16 Mo6 O21 156.0(7) . .
O14 Mo6 O21 86.9(4) . .
O20 Mo6 O21 80.2(5) 2_776 .
O8 Mo6 O4 156.9(5) . 2_776
O16 Mo6 O4 62.9(6) . 2_776
O14 Mo6 O4 99.3(6) . 2_776
O20 Mo6 O4 63.3(5) 2_776 2_776
O21 Mo6 O4 93.2(6) . 2_776
O8 Mo6 O3 155.8(5) . .
O16 Mo6 O3 96.8(7) . .
O14 Mo6 O3 64.0(5) . .
O20 Mo6 O3 93.5(6) 2_776 .
O21 Mo6 O3 63.0(5) . .
O4 Mo6 O3 46.6(4) 2_776 .
O1 Si1 O1 180.000(3) 2_776 .
O1 Si1 O2 109.4(6) 2_776 .
O1 Si1 O2 70.6(6) . .
O1 Si1 O2 70.6(6) 2_776 2_776
O1 Si1 O2 109.4(6) . 2_776
O2 Si1 O2 180.000(7) . 2_776
O1 Si1 O4 70.5(6) 2_776 2_776
O1 Si1 O4 109.5(6) . 2_776
O2 Si1 O4 70.9(6) . 2_776
O2 Si1 O4 109.1(6) 2_776 2_776
O1 Si1 O4 109.5(6) 2_776 .
O1 Si1 O4 70.5(6) . .
O2 Si1 O4 109.1(6) . .
O2 Si1 O4 70.9(6) 2_776 .
O4 Si1 O4 180.000(4) 2_776 .
O1 Si1 O3 69.5(6) 2_776 2_776
O1 Si1 O3 110.5(6) . 2_776
O2 Si1 O3 70.8(6) . 2_776
O2 Si1 O3 109.2(6) 2_776 2_776
O4 Si1 O3 109.0(6) 2_776 2_776
O4 Si1 O3 71.0(6) . 2_776
O1 Si1 O3 110.5(6) 2_776 .
O1 Si1 O3 69.5(6) . .
O2 Si1 O3 109.2(6) . .
O2 Si1 O3 70.8(6) 2_776 .
O4 Si1 O3 71.0(6) 2_776 .
O4 Si1 O3 109.0(6) . .
O3 Si1 O3 180.000(2) 2_776 .
Si1 O1 Mo2 121.9(6) . .
Si1 O1 Mo4 121.7(6) . .
Mo2 O1 Mo4 95.0(4) . .
Si1 O1 Mo1 120.9(6) . .
Mo2 O1 Mo1 95.0(4) . .
Mo4 O1 Mo1 95.6(4) . .
Si1 O2 Mo1 122.3(5) . .
Si1 O2 Mo3 121.7(6) . .
Mo1 O2 Mo3 94.1(4) . .
Si1 O2 Mo5 121.4(6) . 2_776
Mo1 O2 Mo5 95.2(4) . 2_776
Mo3 O2 Mo5 95.2(4) . 2_776
Si1 O3 Mo2 122.3(6) . .
Si1 O3 Mo5 121.1(6) . .
Mo2 O3 Mo5 96.0(4) . .
Si1 O3 Mo6 120.3(6) . .
Mo2 O3 Mo6 96.0(4) . .
Mo5 O3 Mo6 94.6(4) . .
Si1 O4 Mo4 121.6(6) . .
Si1 O4 Mo6 121.8(6) . 2_776
Mo4 O4 Mo6 95.3(5) . 2_776
Si1 O4 Mo3 120.8(7) . 2_776
Mo4 O4 Mo3 95.4(4) . 2_776
Mo6 O4 Mo3 95.3(4) 2_776 2_776
Mo4 O5 Mo1 136.1(7) . .
Mo3 O9 Mo5 137.9(7) . 2_776
Mo1 O10 Mo2 136.1(7) . .
Mo2 O11 Mo4 137.4(7) . .
Mo1 O12 Mo3 135.4(8) . .
Mo5 O13 Mo1 137.1(8) . 2_776
Mo6 O14 Mo2 136.3(8) . .
Mo3 O15 Mo4 136.2(7) . 2_776
Mo6 O16 Mo3 140.8(8) . .
Mo2 O18 Mo5 136.8(7) . .
Mo4 O20 Mo6 135.4(8) . 2_776
Mo5 O21 Mo6 136.3(8) . .
N1 Cu1 N2 174.4(4) . .
C3 N1 C5 116.5(9) . .
C3 N1 Cu1 124.5(9) . .
C5 N1 Cu1 118.7(8) . .
C15 N2 C6 117.0(8) . .
C15 N2 Cu1 119.0(8) . .
C6 N2 Cu1 123.2(8) . .
C10 N3 C14 118(2) . .
C2 C1 C3 117.0(11) . .
C1 C2 C4 117.6(9) . .
C1 C2 C8 123.0(9) . 1_455
C4 C2 C8 119.3(9) . 1_455
N1 C3 C1 126.7(12) . .
C5 C4 C2 119.1(10) . .
N1 C5 C4 123.1(10) . .
N2 C6 C7 123.8(11) . .
C6 C7 C8 118.8(11) . .
C7 C8 C9 117.6(9) . .
C7 C8 C2 122.1(9) . 1_655
C9 C8 C2 120.3(9) . 1_655
C15 C9 C8 119.3(9) . .
N3 C10 C12 123(2) . .
C13 C11 C12 111.8(19) . .
C13 C11 C11 124.8(17) . 2_655
C12 C11 C11 123.2(18) . 2_655
C10 C12 C11 122.4(19) . .
C14 C13 C11 122.8(17) . .
C13 C14 N3 122.3(19) . .
N2 C15 C9 123.4(10) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Mo1 O7 1.666(7) .
Mo1 O12 1.804(10) .
Mo1 O10 1.826(10) .
Mo1 O13 1.995(11) 2_776
Mo1 O5 2.027(9) .
Mo1 O2 2.380(11) .
Mo1 O1 2.414(12) .
Mo2 O6 1.680(7) .
Mo2 O18 1.806(10) .
Mo2 O11 1.827(10) .
Mo2 O14 1.989(10) .
Mo2 O10 1.991(9) .
Mo2 O3 2.356(12) .
Mo2 O1 2.390(12) .
Mo3 O22 1.646(7) .
Mo3 O9 1.803(10) .
Mo3 O15 1.840(10) .
Mo3 O16 1.979(11) .
Mo3 O12 1.979(9) .
Mo3 O4 2.403(12) 2_776
Mo3 O2 2.404(11) .
Mo4 O17 1.654(8) .
Mo4 O20 1.827(12) .
Mo4 O5 1.829(10) .
Mo4 O11 1.973(10) .
Mo4 O15 1.981(10) 2_776
Mo4 O4 2.389(13) .
Mo4 O1 2.413(12) .
Mo5 O19 1.647(8) .
Mo5 O21 1.809(10) .
Mo5 O13 1.810(10) .
Mo5 O18 1.993(9) .
Mo5 O9 2.006(10) 2_776
Mo5 O3 2.398(12) .
Mo5 O2 2.413(12) 2_776
Mo6 O8 1.653(8) .
Mo6 O16 1.787(11) .
Mo6 O14 1.836(11) .
Mo6 O20 1.996(10) 2_776
Mo6 O21 2.008(10) .
Mo6 O4 2.398(13) 2_776
Mo6 O3 2.422(12) .
Si1 O1 1.611(11) 2_776
Si1 O1 1.611(11) .
Si1 O2 1.621(11) .
Si1 O2 1.621(11) 2_776
Si1 O4 1.639(12) 2_776
Si1 O4 1.639(12) .
Si1 O3 1.642(12) 2_776
Si1 O3 1.642(12) .
O2 Mo5 2.413(12) 2_776
O4 Mo6 2.398(13) 2_776
O4 Mo3 2.403(12) 2_776
O9 Mo5 2.006(10) 2_776
O13 Mo1 1.995(11) 2_776
O15 Mo4 1.981(10) 2_776
O20 Mo6 1.996(10) 2_776
Cu1 N1 1.898(8) .
Cu1 N2 1.901(8) .
N1 C3 1.282(17) .
N1 C5 1.341(16) .
N2 C15 1.333(15) .
N2 C6 1.340(16) .
N3 C10 1.29(3) .
N3 C14 1.36(3) .
C1 C2 1.390(14) .
C1 C3 1.393(15) .
C2 C4 1.397(15) .
C2 C8 1.475(12) 1_455
C4 C5 1.387(14) .
C6 C7 1.389(14) .
C7 C8 1.392(14) .
C8 C9 1.393(14) .
C8 C2 1.475(12) 1_655
C9 C15 1.391(13) .
C10 C12 1.33(3) .
C11 C13 1.41(2) .
C11 C12 1.42(3) .
C11 C11 1.44(4) 2_655
C13 C14 1.29(3) .
